ISSN: 2087-3948 (print. ISSN: 2087-3956 (electronic.
Vol. 3, No. 2, Pp. 59-63 July 2011
A biogenic approach for green synthesis of silver nanoparticles using extract of Foeniculum vulgare and its activity against Staphylococcus aureus and Escherichia coli SHITAL BONDE♥ Department of Biotechnology, SGB Amravati University, Amravati 444602, Maharashtra, India. Tel: +91-721-2662207/8, Extension-267. Fax: +91 721 2660949, 2662135, ♥email: [email protected]
Manuscript received: 10 May 2011. Revision accepted: 7 June 2011.
Abstract. Bonde S. 2011. A biogenic approach for green synthesis of silver nanoparticles using extract of Foeniculum vulgare and its activity against Staphylococcus aureus and Escherichia coli. Nusantara Bioscience 3: 59-63. We report green synthesis of silver nanoparticles from extract of Foeniculum vulgare (fennel, saunf). The synthesis of silver nanoparticles was detected by changing color from green to brown after treatment with AgNO3 (1mM) and the UV-visible spectrophotometer analysis showed the absorbance peak at about 427 nm, which indicates the synthesis of silver nanoparticles. Nanoparticle Tracking and Analysis (NTA) by LM-20 was used for multi-parameter analysis, allowing for characterization of particle size and particle distribution of silver nanoparticles synthesized from extract of F. vulgare. NTA revealed the polydispersed nanoparticles in the range of 18-83 nm. Phytosynthesized silver nanoparticles showed antibacterial activity against the Staphylococcus aureus (ATCC-25923) and Escherichia coli (ATCC-39403). The silver nanoparticles also demonstrated remarkable antibacterial activity against two human pathogenic bacteria when used in combination with commercially available antibiotics. The bactericidal activity of the standard antibiotics was significantly enhanced in presence of silver nanoparticles against pathogenic bacteria, viz. E. coli-JM-103 (ATCC-39403) and S. aureus (ATCC-25923). Silver nanoparticles in combination with vancomycin showed maximum activity against E. coli (increase in fold area 5.76. and followed by S. aureus (1.08) and Gentamicin showed the maximum activity S. aureus (2.6) while E. coli (0.96). The approach of phytosynthesized silver nanoparticles using F. vulgare appears to be cost efficient, eco-friendly and easy alternative to conventional methods of synthesis. Key words: Foeniculum vulgare, silver nanoparticles, LM20, antibacterial.
Abstrak. Bonde S. 2011. Pendekatan biogenik untuk sintesis nanopartikel perak menggunakan ekstrak Foeniculum vulgare dan aktivitasnya terhadap Staphylococcus aureus dan Escherichia coli. Nusantara Bioscience 3: 59-63. Kami melaporkan sintesis nanopartikel perak dari ekstrak Foeniculum vulgare (adas). Sintesis nanopartikel perak terdeteksi dengan mengubah warna dari hijau sampai coklat setelah perlakuan dengan AgNO 3 (1mm); dan analisis spektrofotometer UV-vis menunjukkan puncak absorbansi pada sekitar 427 nm, yang menunjukkan sintesis nanopartikel perak. Analisis Pelacakan Nanopartikel (NTA) oleh LM-20 digunakan untuk analisis multi-parameter, memungkinkan untuk karakterisasi ukuran partikel dan distribusi partikel nanopartikel perak yang disintesis dari ekstrak F. vulgare. NTA mengungkapkan nanopartikel tersebar di kisaran 18-83 nm. Fitosintesis nanopartikel perak menunjukkan aktivitas antibakteri terhadap Staphylococcus aureus (ATCC-25923) dan Escherichia coli (ATCC-39403). Perak nanopartikel juga menunjukkan aktivitas antibakteri yang luar biasa terhadap dua bakteri patogen manusia apabila digunakan dalam kombinasi dengan antibiotik yang tersedia secara komersial. Aktivitas bakterisida antibiotik standar secara signifikan ditingkatkan dengan adanya nanopartikel perak terhadap bakteri patogen, yaitu: E. coli-JM-103 (ATCC-39403) and S. aureus (ATCC-25923). Nanopartikel perak yang dikombinasi dengan vankomisin menunjukkan aktivitas maksimal terhadap E. coli (kenaikan berlipat 5,76) dan diikuti oleh S. aureus (1,08); dan gentamisin menunjukkan aktivitas maksimum S. aureus (2,6) sedangkan E. coli (0,96). Pendekatan fitosintesis nanopartikel perak menggunakan F. vulgare tampaknya memerlukan biaya yang efisien, ramah lingkungan dan merupakan alternatif mudah untuk metode sintesis konvensional. Kata kunci: Foeniculum vulgare, nanopartikel perak, LM20, antibakteri.
INTRODUCTION Phytosynthesis at present seems to be the biological method of much interest (Safaepour et al. 2009). Phytosynthesis is better compared to microorganisms because the later suffer from various problems like culture maintenance and cost effectiveness during the scale up process. Various plants have been successfully used for the synthesis of biogenic metal nanoparticles (Singh et al. 2011).
The rapid synthesis of silver nanoparticles by biological method using plant extracts of Pinus, Persimmon, Ginkgo, Magnolia and Platanus were used and compared for their extracellularly metallic silver nanoparticles (Song et al. 2008) and the utilization of Azadirachta indica (neem). (Shankar et al. 2004), Medicago sativa (alfalfa), Aloe vera (Chandran et al. 2006), Emblica officinalis (amla). (Amkamwar et al. 2005), Capsicum annuum (Li et al. 2007), Cinnamomum
3 (2): 59-63, July 2011
camphora (Huang et al. 2007), Gliricidia sepium Jacq. (Raut et al. 2009), Carrica papaya (Mude et al. 2009), Opuntia ficus-indica (Gade et al. 2010), Murraya koenigii (Bonde et al. 2010), Ocimum sanctum (Mallikarjum et al. 2011), Saururus chinenis (Nagajyoti et al. 2011), and microorganisms (Duran et al. 2005; Bhainsa et al. 2006) has been reported fennel (Foeniculum vulgare) is an important crop plant with medicinal value being carminative. Its fruits are used as a digestive adjuvant having antimicrobial activity (He and Huang 2011). The multi-drug resistant pathogens are responsible for causing death worldwide (Bandow et al. 2003; Wright et al. 2005) and hence there is a pressing need for the development of novel antimicrobial agents. Reports suggest that silver nanoparticles can be used effectively against multi-drug resistant bacteria (Ingle et al. 2008) due to their small size and relatively large surface area in comparison to their volume makes easy to interact with substances and increases their antibacterial efficacy. Silver nanoparticles are the new generation of antimicrobials (Rai et al. 2009) and it can be used in many antimicrobial preparations. Gade et al. (2008. and Ingle et al. (2008) reported the antibacterial activity of silver nanoparticles synthesized by fungi. Antibacterial activity of silver nanoparticles synthesized by leaf broth of Gliricidia sepium was reported by Raut et al. (2009). Duran et al. (2007) successfully developed silver nanoparticle impregnated wound dressings and textile fabrics which can be used for burnt patients. Silver nanoparticles are also used for the preparation of surgical masks (Li et al. 2006). In the present study, F. vulgare was used for the synthesis of silver nanoparticles and the activity of synthesized silver nanoparticles was evaluated against S. aureus and E. coli in combination with commercially available five antibiotics viz. gentamicin, oxacillin, vancomycin, ampicillin and amoxycillin, to study synergistic effect, if any.
MATERIALS AND METHODS The test plant The young and healthy leaves of Foeniculum vulgare were collected from the field of Department of Biotechnology, Sant Gadge Baba Amravati University, Amravati, Maharashtra State, India. Test bacteria Escherichia coli-JM-103 (ATCC-39403) and Staphylococcus aureus (ATCC-25923) were used to evaluate the activity of silver nanoparticles in combination with standard antibiotics (viz. gentamicin, oxacillin, vancomycin, ampicillin and amoxycillin, purchased from Himedia). Extraction The leaves of F. vulgare (20 g) were washed twice in tap water and rinsed thrice in distilled water. Then surface sterilized by HgCl2 (0.1%) for 1 min, cut into small pieces and crushed with 100 mL of sterilized distilled water in an Omni mixer. Later, crude extract was filtered through muslin cloth and centrifuged at 10,000 rpm for 15 min to
obtain clear leaf extract which was later used for the synthesis of silver nanoparticles. Synthesis of silver nanoparticles For the synthesis of silver nanoparticles leaf extract was challenged with AgNO3 (1mM) solution and incubated at room temprature. Control (without treatment with AgNO3. (1mM) i.e. only leaf exrtact) was also maintained. After the reduction of aqueous silver ions into silver nanoparticles, residual silver ions (unreacted silver ions) were removed from the reaction mixture by centrifugation and presence of unreacted silver ions were detected by the treatment with sodium chloride (NaCl) as a result white precipitate of silver chloride (AgCl) was formed after reacting with Ag+ ion. Triplicates of each treatment were maintained. Detection and characterization of silver nanoparticles Visual observation. After treatment of leaf extract with AgNO3 (1mM), the colour change of the reaction mixture was visually observed. UV-Vis spectrophotometric analysis. The aliquotes of reaction mixture were subjected to the meausurement of absorbance by UV-visible spectrophotometer (Perkin Elmer, Labda-25. at a resolution of 1 nm from 250 to 800 nm for the detection of silver nanoparticles. NanoSight LM-20 analysis. Liquid sample of silver nanoparticles at the concentration range of 107-109/mL were introduced into a scattering cell through which a laser beam (approx. 40 mW at k = 635 nm) was passed. Particles present within the path of the laser beam were observed via a dedicated non-microscope optical instrument (LM-20, NanoSight Pvt. Ltd., UK. having CCD camera. The motion of the particles in the field of view (approx. 100 X 100 μm) was recorded (at 30 fps) and the subsequent video and images were analyzed. Each particle visible in the image is individually but simultaneously traced from frame to frame, the mean square displacement is determined by analytical programme. Particle size measurement. Particle sizing experiments were carried out by means of laser diffractometry, using Zetasizer nano series (Malvern) Measurements were taken in the range range between 0.1-1000µm. Assessment of antibacterial activity The disc diffusion method was used to evaluate the antibacterial potential of silver nanoparticles and combined effect of silver nanoparticles with five antibiotics against two human pathogenic bacteria: E. coli-JM-103 (ATCC39403) and S. aureus (ATCC-25923) grown on nutrient agar plates. The overnight grown bacterial culture having 105 CFU/mL was used to assess the activity. The test bacterial cultures were inoculated on to solidified agar plates. The different standard antibiotic discs (viz. gentamicin, oxacillin, vancomycin, ampicillin and amoxycillin) purchased from Hi-Media, Mumbai were used. To evaluate the combined effects, each standard antibiotic disc impregnated with 20 µL solution of silver nanoparticles was placed on to the agar surface inoculated with test bacteria. The plates were then incubated at 370C for 24 hours. After incubation, the zones of inhibition were
BONDE-Synthesis of silver nanoparticles using extract of Foeniculum vulgare
measured and its activities were evaluated by calculating the increase in fold-area. The assays were performed in triplicate. Assessment of increase in fold area The increase in fold area was assessed by calculating the mean surface area of the inhibition zone of each tested antibiotic. The fold increase area of different antibiotics was calculated by using the equation calculated as (b2-a2) ⁄ a2, where a and b are the inhibition zones for A and B, respectively. In the same way, c and d.
Huang et al. (2007) and Li et al. (2007) reported the similar results, observed that when sun dried leaf extract of Cinnamomum camphora and Capsicum annuum were challenged with aqueous silver ions, the reaction mixture containing silver nanoparticles showed the absorption peak at about 427 nm due to the excitation of plasmon resonance vibration.
RESULTS AND DISCUSSION The synthesis of silver nanoparticles by leaf extract of F. vulgare was performed in the present study. On treatment of leaf extract with AgNO3 (1mM) and incubated in dark at room temperature, within 1 hour of the reaction, colour changes from green to brown (Figure 1) indicating the synthesis of silver nanoparticles. It is an efficient and rapid method of synthesis which corroborate with the results obtained by other researchers who worked with different plant systems (Shankar et al. 2004; Chandran et al. 2006; Li et al. 2007; Mallikarjun et al. 2011). Colour change was due to the excitation of surface plasmon vibrations in the metal nanoparticles (Ahmad et al. 2003).
Figure 1. Control (left) and silver (right) nanoparticles synthesized from Foeniculum vulgare
UV-Vis spectrophotometric analysis has proved to be a very useful technique for the analysis of nanoparticles. In order to verify the synthesis of silver nanoparticles, the test samples were subjected to UV-Vis spectrophotometric analysis. The test samples (leaf extract treated with 1mM silver nitrate. were collected in aliquots from the reaction mixture and analyzed to record their absorbance by UV-Vis spectrophotometer. This analysis showed the sharp absorbance at around 427 nm in the form of peak (Figure 2), which was specific for silver nanoparticles (Shankar et al. 2004; Chandran et al. 2006; Elumalai et al. 2010).
Figure 2. UV-Visible spectroscopy of synthesized silver nanoparticles from Foeniculum vulgare
Here we demonstrated Nanoparticle Tracking and Analysis (NTA) to measure the dispersion characteristics i.e. size and size distribution on their brownian motion in suspension. NTA allows individual nanoparticles in a suspension to be microscopically visualized and their brownian motion to be separately but simultaneously analyzed and from which the particle size distribution can be obtained on a particle-by-particle basis which enables separation of particle population by size and intensity. The NTA showed particle populations by size and intensity. These results correlates the results obtained by MontesBurgos and group (Montes-Burgos et al. 2010). Total Concentration of silver nanoparticles synthesized by leaf extract of F. vulgare was found to be 7.6 particles/frame, 3.35X108 particles/mL. The size of silver particle analyzed by NTA was in the range of 18-83 nm. Statistical distribution of silver nanoparticles using LM 20, mean: 82nm, mode: 83 nm. SD: 25 nm. Distribution of Particle Size/Concentration of Ag NPs was showed in Figure 3a and the particle populations of Ag NPs using NanoSight LM-20 were studied (Figure 3a and 3b). Particle size determination of the formulated nanoparticles was shown under different categories like size distribution by volume, by intensity (Figure 4). First and second peaks, the average diameter of the particles were found to be 127, 100% and width 37.25 nm. The formed silver nanoparticles are well distributed with respect to volume and intensity is an indication of the formation of well built silver nanoparticles and their monodispersity.
Figure 3a. Particle Size / Concentration of Ag NPs
3 (2): 59-63, July 2011
Figure 3b. Particle populations of Ag NPs using NanoSight LM20.
Figure 4. Particle size distribution of Ag-NPs by intensity with Zeta Analyzer. Table 1. Comparison in increase in fold area zone of activity of different antibiotics against S. aureus, and E. coli (in absence and in presence of silver nanoparticles (AgNPs) at concentration of 20µl/disc. (Where, Ab= Antibiotics, Ab+ Ag-NPs= Antibiotics + silver nanoparticles) Staphylococcus aureus Ab Ab+ *Increase Antibiotics (A) Ag-NPs in fold (B) area Gentamicin 19 ± 0.3 36±0.1 2.6±0.2 Oxacillin 24± 0.2 29±0.3 0.32±0.3 Vancomycin 18 ± 0.4 26±0.4 1.08±0.2 Ampicillin 27 ± 0.1 31±0.2 0.31±0.1 Amoxycillin 29 ± 0.2 32±0.1 0.21±0.3 Note: Inhibition zone in mm
Escherichia coli Ab+ *Increase Ab Ag-NPs in fold (C) (D) area 20±0.3 28±0.4 0.96 28±0.5 30±0.1 0.14 10±0.1 26±0.2 5.76 21±0.2 24±0.4 0.31 19±0.2 25±0.3 0.73
We report synthesis of silver nanoparticles by F. vulgare for the first time as there is no report of synthesis of silver nanoparticles by this plant. Moreover, the phytosynthesized silver nanoparticles were used for the evaluation of their antibacterial efficacy in combination with commercially available antibiotics. From the present study, it was observed that the efficacy of silver nanoparticles against test bacteria (E. coli and S. aureus) was increased when assessed in combination of antibiotics. It is evidenced by the data provided in Table 1, which showed increase in activity fold area for each antibiotic. The bactericidal activity of the standard antibiotics was significantly increased in presence of silver nanoparticles against pathogenic bacteria, viz. E. coli-JM-103 (ATCC39403) and S. aureus (ATCC-25923) Silver nanoparticles in combination with Vancomycin showed maximum activity against E. coli (increase in fold area 5.76) and S. aureus (1.08) and gentamicin showed the maximum activity S. aureus (2.6) while E. coli (0.96). While other antibiotics did not show significant inhibitory activity against the test bacteria. These findings support the report by Birla et al. 2009 year, who reported that the activity of commercially available antibiotics with silver nanoparticles synthesized by a
BONDE-Synthesis of silver nanoparticles using extract of Foeniculum vulgare
fungus Phoma glomerata was more against Gram-negative bacteria compared to the Gram-positive bacteria and also Savitthramma et al. (2011) report the silver nanoparticles of Boswellia avalifoliota showed maximum inhibition of E. coli. The green method of synthesis is safer than other. There are three types of antimicrobial mechanisms observed by Song et al. (2006), i.e. (i) Plasmolysis, cytoplasm of bacteria separated from bacterial cell wall, was observed in Gram negative bacteria and Gram positive bacteria, (ii) inhibited cell wall synthesis and (iii) induces metabolic disturbances to pathogenic bacteria.
CONCLUSION The present study included the bioreduction Ag + ions by plant F. vulgare and its antibacterial activity. The study reveals that plant species are good and fast rate source of synthesis and the antibacterial efficacy against S. aureus and E. coli confirmed that the silver nanoparticles are capable of rendering antibacterial efficacy and strengthen the medicinal value of plants. Phytosynthesis of silver nanoparticles are most convenient, easily scale up and ecofriendly.
ACKNOWLEDGEMENTS The author is grateful to Prof. M.K. Rai and A.K. Gade for their guidance and support. Author wishes to thank S.C. Gaikwad for helping in analysis of LM20, and to Funds for Infrastructure Science and Technology (FIST. for providing computer facility, Department of Biotechnology, S.G.B.A.U. Amravati and Prof. Nelson Duran, Department of Biological Chemistry, University of Campinas, Brazil for providing Zeta analyzer instrument facility.
REFERENCES Ahmad A, Mukherjee P, Senapati S, Mandal D, Khan MI, Kumar R. 2003. Extracellular biosynthesis of silver nanoparticles using the fungus Fusarium oxysporum. Coll Surf B 28: 313-318. Amkamwar B, Damle C, Ahmad A, Sastry M. 2005. Biosynthesis of gold and silver nanoparticles using Emblica officinalis fruit extract, their phase transfer and transmetallation in an organic solution. J Nanosci Nanotechnol 5: 1665-1671. Bandow JE, Brotz H, Leichert LIO, Labischinski H, Hecker M. 2003. Proteomic approach to understanding antibiotic action. Antim Agents Chem 47: 948-955. Bhainsa KC, D'Souza SF. 2006. Extracellular biosynthesis of silver nanoparticles using the fungus Aspergillus fumigatus. Colloids Surf B Biointerfaces 47: 160-164. Birla SS, Tiwari VV, Gade AK, Ingle AP, Yadav AP, Rai MK. 2009. Fabrication of silver nanoparticles by Phoma glomerata and its combined effect against Escherichia coli, Pseudomonas aeruginosa and Staphylococcus aureus. Lett App Microbiol 48: 173-179. Bonde SR, Rathod DP, Ingle AP, Ade RB, Gade AK, Rai MK. 2010. Murraya koenigii mediated synthesis of silver nanoparticles and its activity against three human pathogenic bacteria. J Exp Nanosci (in press).
Chandran SP, Chaudhary M, Pasricha R, Ahmad A, Sastry M. 2006. Synthesis of gold nanotriangles and silver nanotriangles using Aloe vera plant extract. Biotech Prog 22: 577-579. Duran N, Marcarto PD, De Souza GIH, Alves OL, Esposito E. 2007. Antibacterial effect of silver nanoparticles produced by fungal process on textile fabrics and their effluent treatment. J Biomed Nano 3: 203208. Duran N, Marcato PD, Alves OL, Souza GI, Esposito E. 2005. Mechanistic aspects of biosynthesis of silver nanoparticles by several Fusarium oxysporum strains. J Nanobiotechnol 3: 8. Elumalai EK, Prasad TN, Kambala , Nagaiyothi PC, David E. 2010. Green synthesis of silver nanoparticle using Euphorbia hirta L and their antifungal activities. Arch Appl Sci Res 2 (6): 76-81 Gade AK, Bonde P, Ingle AP, Marcato PD, Duran N, Rai, MK. 2008. Exploitation of Aspergillus niger for synthesis of silver nanoparticles. J Biobased Mat Bioengineer 2: 243-247. Gade AK, Gaikwad SC, Tiwari V, Yadav A, Ingle AP, Rai MK. 2010. Biofabrication of silver nanoparticles by Opuntia ficus-indica: In vitro antibacterial activity and study of the mechanism involved in the synthesis. Curr Nanosci 6: 370-375. He W, Huang B. 2011. A review of chemistry and bioactivities of a medicinal spice: Foeniculum vulgare. J Med Pl Res 5 (16): 35953600 Huang J, Chen C, He N, Hong J, Lu Y, Qingbiao L, Shao W, Sun D, Wang Y, Wang XH, Yiang X. 2007. Biosynthesis of silver and gold nanoparticles by novel sun dried Cinnamomum camphora leaf. Nanotechnol 18: 105-106. Ingle A, Gade A, Pierrat S, Sonnichsen C, Rai M. 2008. Mycosynthesis of silver nanoparticles using the fungus Fusarium acuminatum and its activity against some human pathogenic bacteria. Curr Nanosci 4: 141-144. Li LP, Song QW, Newton E. 2006. Antimicrobial effects of surgical masks coated with 869 nanoparticles. J Hosp Infect 62: 58-63. Li S, Qui L, Shen Y, Xie A, Yu X, Zhang L, Zhang Q. 2007. Green synthesis of silver nanoparticles using Capsicum annum L. extract. Green Chem 9: 852-858. Mallikarjun K, Narsimha G, Dillip GR, Praveen B, Shreedhar B, Lakshmi S, Reddy VS, Raju DP. 2011. Green synthesis of silver nanoparticles using Ocimum leaf extract and their characterization. Digest J Nanomat Biostruct 6 (1): 181-186. Mude N, Ingle A, Gade A, Rai M. 2009. Synthesis of silver nanoparticles using callus extract of Carica papaya-A first report. J Pl Biochem Biotechnol 18: 83-86. Nagajyoti PC, Prasad TN, Shreekanth VM, Lee KD. 2011. Biofabrication of silver nanoparticles using leaf of Saururus chinenis. Digest J Nanomat Biostruct 6 (1): 121-133. Rai MK, Yadav AP, Gade AK. 2009. Silver nanoparticles as a new generation of antimicrobials .Biotech Adv 27 (1): 76-82. Raut RW, Lakkakula JR, Kolekar NS, Mendhulkar VD, Kashid SB. 2009. Phytosynthesis of silver nanoparticle using Gliricidia sepium (Jacq.). Curr Nanosci 5: 117-122. Safaepour M,Shahaverdi AR, Shaverdi HR, Khorramizadeh MR, Gohari AR. 2009. Green Synthesis of small silver nanoparticles using geraniol and its cytotoxicity against Fibrosarcoma-Wehi 164. Avicenna J Med Biotech 1 (2): 111-115. Savittramma N, Rau LM, Suvarnalatha P. 2011. Evaluation of antibacterial efficacy of biological synthesized silver nanoparticles using stem barks of Boswellia avalifoliolata Bal. and Henry and Shorea tumbuggaia Roxb. J Biol Sci 11 (1): 39-45. Shankar SS, Rai A, Ahmad A, Sastry MJ. 2004. Rapid synthesis of Au, Ag, and bimetallic Au core-Ag shell nanoparticles using Neem (Azadirachta indica) leaf broth. J Colloid Interface Sci 275: 496-502. Singh C, Sharma V, Naik PK, Khandelwal V, Singh H. 2011. A green biogenic approach for synthesis of gold and silver nanoparticles using Zingiber officinale. Digest J Nanomat Biostruct 6 (2): 535-542. Song H.Y, Ko KK, Oh IH, Lee BT. 2006. Fabrication of silver nanoparticles and their antimicrobial mechanisms. Eur Cells Mater 11 (1): 58. Song JY, Beom SK. 2008. Rapid biological synthesis of silver nanoparticles using plant leaf extracts. Bioproc Biosyst Engineer 32 (1): 79-84. Wright GD. 2005. Bacterial resistance to antibiotics: Enzymatic degradation and modifications. Adv Drug Del Rev 57: 1451-1470.